Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

- Thermal power plant1 by Nikhil Kumar 563 views
- STRUCTURE DESIGN AND ANALYSIS OF HY... by NISHANTH H D 265 views
- Stress analysis. by Basel Saleh 297 views
- Renewable Vs Non-Renewable Energy (... by newaz30 2271 views
- Ch04 section15 pressure_vessel_design by Paralafakyou Mens 734 views
- A presentation on steam power plant1 by Sant Longowal Ins... 2500 views

1,243 views

Published on

No Downloads

Total views

1,243

On SlideShare

0

From Embeds

0

Number of Embeds

2

Shares

0

Downloads

27

Comments

0

Likes

1

No embeds

No notes for slide

- 1. 2012 American Transactions on Engineering & Applied Sciences American Transactions on Engineering & Applied Sciences http://TuEngr.com/ATEAS, http://Get.to/Research Computer Modeling of Internal Pressure Autofrettage Process of a Thick-Walled Cylinder with the Bauschinger Effect a* a Zhong Hu , and Sudhir Puttaguntaa Department of Mechanical Engineering, South Dakota State University, USAARTICLEINFO A B S T RA C TArticle history: In this paper, the internally pressure overloading autofrettageReceived January 13, 2012Accepted January 27, 2012 process of a thick-walled cylinder has been numerically investigated.Available online The corresponding axi-symmetric and plane-stress finite elementJanuary, 28 2012 model has been employed. The elasto-plastic material model withKeywords: nonlinear strain-hardening and kinematic hardening (the BauschingerThick-walled cylinder; effect) was adopted. The residual stresses in the thick-walled cylinderInternal Pressurize; induced by internal autofrettage pressure have been investigated andAutofrettage; optimized. The optimum autofrettage pressure and the maximumBauschinger effect;Finite Element Analysis reduction percentage of the von Mises stress in the autofrettaged thick-walled cylinder under the elastic-limit working pressure have been found, the differences of stress and strain distribution between adopting the Bauschinger-effect and the non-Bauschinger-effect have been compared. 2012 American Transactions on Engineering & Applied Sciences.1. Introduction Thick-walled cylinders subjected to high internal pressure and/or elevated temperature arewidely used in the nuclear and chemical industries involving pressures as high as 1380 MPa and*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 143http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 2. temperatures of up to 300 °C, (Ford et al. 1981) especially for military applications involvingtransient peak internal pressures as high as 350 MPa and temperature of up to 1500 °C inside thegun barrel in a ballistic event. (Bundy et al. 1996) In the absence of residual stresses, cracks usuallyform at the bore where the hoop stress developed by the working pressure is highest. (Daniels1942; Zapfec 1942; Bush 1988; Masu and Graggs 1992) To prevent such failure and to increase thepressure-carrying capacity, a common practice is autofrettage treatment of the cylinder prior to use.Autofrettage is used to introduce advantageous favorable compressive residual hoop stress insidewall of a cylinder and result in an increase in the fatigue lifetime of the component. There arebasically three types of autofrettage. These are carried out by hydraulic pressurization, bymechanically pushing an oversized mandrel, or by the pressure of powder gas, (Davidson andKendall 1970; Malik and Khushnood 2003) in which hydraulic and powder gas pressurization arebased on the same principal and strengthening mechanism. In general, vessels under high pressurerequire a strict analysis for an optimum design for reliable and secure operational performance.Prediction of residual stress field and optimization of the autofrettage processes’ parameters aresome of the key issues in this context, which normally involve a careful evaluation of the relatedmodeling, simulation and experimental details. (Davidson et al. 1963; Chu and Vasilakis 1973;Shannon 1974; Tan and Lee 1983; Gao 1992; Avitzur 1994; Kandil 1996; Lazzarin and Livieri1997; Zhu and Yang 1998; Venter et al. 2000; Gao 2003; Iremonger and Kalsi 2003; Kihiu et al.2003; Parker et al. 2003; Perry and Aboudi 2003; Zhao et al. 2003; Perl and Perry 2006; Bihamta etal. 2007; Hojjati and Hassani 2007; Korsunsky 2007; Gibson 2008; Perry and Perl 2008; Ayob etal. 2009; Darijani et al. 2009) Efforts are continually made in the regarding aspects. Overloading pressure autofrettage process involves the application of high pressure to theinner surface of a cylinder, until the desired extent of plastic deformation is achieved. Analyticalsolution of pressure autofrettage of a constant cross-section cylinder, subject to some endconditions, is possible through the use of simplifying assumptions, such as choice of yield criteriaand material compressibility and, critically, material stress-strain behavior. On the other hand,autofrettage causes large plastic strains around the inner surface of a cylinder, which noticeablycauses the early onset of non-linearity when remove the autofrettage pressure in the unloadingprocess – a kinematic hardening phenomenon termed the Bauschinger effect. This non-linearitytypically causes significant deviation from those material models that are often assumed. The effectis most pronounced around the inner surface, and in turn has a significant effect on the residual 144 Zhong Hu, and Sudhir Puttagunta
- 3. stresses developed when the autofrettage load is removed, especially as it can cause reverseyielding to occur when it otherwise would not be expected. Research has been done on this issuewith theoretical analysis mostly based on bilinear kinematic hardening (linear elastic and linearhardening) material model which is a good approximation for small strain. (Lazzarin and Livieri1997; Venter et al. 2000; Kihiu et al. 2003; Parker et al. 2003; Perry and Aboudi 2003; Huang 2005;Perl and Perry 2006; Korsunsky 2007). However, the practical material model is of nonlinearkinematic hardening and with equivalent strain up to 0.5~1% in the autofrettage process, whichgives complexity to theoretical analysis using nonlinear kinematic hardening material model. Inthis paper, the internally pressure overloading autofrettage process will be numericallyinvestigated. An axi-symmetric and plane stress (for open-ended cylinder) finite element modelwill be presented. The elasto-plastic nonlinear material constitutive relationship will be adopted,incorporating a nonlinear kinematic hardening (the Bauschinger effect) for which no analyticalsolution exists. The effects of the autofrettage pressure on the residual stresses in a thick-walledcylinder will be evaluated. The percentage of stress reduction by autofrettage treatment will becalculated based on von Mises yield criterion. The optimum autofrettage pressure will be found.The differences of stress and strain distribution between adopting the Bauschinger-effect and thenon-Bauschinger-effect will be compared.2. Mathematical Model In this work, the thick-walled cylinder is made of stainless steel AISI 304. An elasto-plasticgoverning equations for material behavior with a homogeneous and isotropic hardening model isused. The true stress – true strain behavior of the strain hardening material follows the Hooke’s lawin the elastic region, and, for comparison purpose, the power-law hardening in the plastic region,(Hojjati and Hassani 2007) (1),where σ and are true stress and true strain, respectively. is the strain at the yield point. E isthe modulus of elasticity. K is a material constant equal to , and n is thestrain-hardening exponent of the material (0 ≤ n < 1). σy is the yield stress. Table 1 lists the basic*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 145http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 4. parameters and material data and derived material parameters to be used in the FEA modeling.(Peckner and Bernstein 1977; Harvey 1982; Boyer et al. 1985; ASM International HandbookCommittee 1990). Figure 1 shows the elasto-plastic stress-strain relationship with kinematichardening (the Bauschinger effect). Commercially available software ANSYS has been used forfinite element modeling of the autofrettaged thick-walled cylinder. (Swanson Analysis System Inc.2011) The finite element model is shown in Figure 2. The element PLANE183 with the capacity ofelastic and plastic material nonlinearity and non-linear kinematic hardening (theBauschinger-effect) has been adopted, which is an eight-node plane-stress 2-D element with higheraccuracy quadratic shape function. In order to get reasonable accuracy, more elements are usednear inner surface and outer surface of the cylinder, see Figure 2. Table 1: Model dimensions and material properties. Material of the Cylinder AISI304 Modulus of Elasticity E 196.0 GPa Poissons Ratio υ 0.29 Yield Strength 152.0 MPa* Strain at Yield Point 7.755×10-4 Strain-Hardening Exponent n 0.2510 Material Constant K 917.4 MPa Inner Radius a 60 mm Outer Radius b 90 mm Maximum Working Pressure pi 47.22MPa * corresponding to 215MPa at 0.2% offset and ultimate tensile strength of 505 MPa. Figure 1: The elasto-plastic stress – strain model with kinematic hardening (the Bauschinger effect). 146 Zhong Hu, and Sudhir Puttagunta
- 5. Figure 2: Finite element model of a plane-stress thick-walled cylinder.3. Modeling Results and Discussions Consider a thick-walled cylinder having inner radius a and outer radius b and subjected to theinternal pressure pi as shown in Figure 2. The material will obey the Hooke’s law when it is withinthe elastic region. This allow us to use the Lame’s equations for calculating the hoop stress, , andradial stress, , along the thickness of the cylinder, when the ends of the cylinder are open andunconstrained so that the cylinder is in a condition of plane stress. (Ugural 2008) 1 (2), 1 (3), 0 (4), Therefore, the von Mises (equivalent) stress is 1 3 (5), The radial displacement is*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 147http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 6. 1 1 (6), Obviously, the maximum von Mises stress is at r = a. Assuming von Mises yield criterionapplied, i.e., , so by substituting the data from Table 1, the maximum applied workingpressure (the maximum internal pressure without causing yielding) is 1 3 47.2 (MPa) (7), Figure 3 shows the analytical and modeling results of stress components and radialdisplacement along the thickness of the cylinder subjected to the maximum working pressure (pwmax = 47.2 MPa). The modeling results are well agreed with the analytical results from Lame’sequations, indicating the reliability of the model employed in the numerical analysis. Figure 3 alsoshows that the maximum von Mises stress and hoop stress located at the inner surface of thecylinder, and the hoop stress is the major stress component causing yield failure. 1.2 4.2E‐5 σθ/σy by Eq.(2) σθ/σy by Modeling 1 σr/σy by Eq.(3) 4.1E‐5 σr/σy by Modeling Displacement u (m) 0.8 σi /σy by Eq.(5) 4.0E‐5 σi/σy by Modeling Stress Ratio σ/σy u by Eq.(6) 0.6 3.9E‐5 0.4 3.8E‐5 0.2 3.7E‐5 0 3.6E‐5 0 20 40 60 80 100 ‐0.2 3.5E‐5 ‐0.4 3.4E‐5 (r‐a)/(b‐a)×100 (%)Figure 3: Analytical and modeling results of stresses and radial displacement along the thickness of the cylinder subjected to the maximum working pressure (pw max = 47.2 MPa). 148 Zhong Hu, and Sudhir Puttagunta
- 7. 1.6 Autofrettage Pressure Ratio 1.5 1.4 pa/pwmax 1.3 1.2 pa/pw max by Eq.(8) from Refs. (Gao 1992 and 2003) 1.1 pa/pw max by Modeling 1 0 20 40 60 80 100 Elasto‐plastic interface (ρ‐a)/(b‐a)*100 (%) Figure 4: The relationship of elastic-plastic interface ρ and the autofrettage pressure pa. As the internal pressure increasing, yielding (plastic deformation) starts from cylinder’s innersurface and gradually extends towards cylinder’s outer surface. This process is basically anelastic-plastic deformation process. The relation between internal autofrettage pressure, pa, and theradius of the elastic-plastic boundary (interface) in plane stress condition, ρ, is determined by (Gao1992; Gao 2003) √ cos , √ / √ (8), , / √ cos ,Where √ cos (9), √ During autofrettage process, the elastic-limit pressure pe (pressure at which yieldingcommences at inner surface) is obviously 1 and in the given case, and theplastic-limit pressure py (pressure at which plasticity has spread throughout the cylinder) is*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 149http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 8. 1.543 and in the given case. Figure 4 shows the relation of elastic-plastic interfaceρ and the autofrettage pressure pa obtained by modeling and analytical approaches, they are wellagreed. Figures 5-7 show the autofrettage stress distributions for the thick-walled cylinder subjected todifferent internal autofrettage pressure range of 1~1.6 by modeling. Hoop stress andvon Mises stress in Figures 5 and 7 clearly indicate that by increasing applied autofrettage pressure,elastic-plastic interface (the turning point of the curve corresponding to the position ρ in Figure 4)moves towards the outer surface of the cylinder and eventually reaches the outer surface, whileradial stress in Figure 6 indicate that the radial stress in compression, with highest compressivestress in the inner surface and zero in the outer surface, increasing as the autofrettage pressureincreasing. 1.1 1.0 Autofrettage Hoop Stress Ratio σaθ/σy 0.9 0.8 0.7 by Modeling under pw max 0.6 by Modeling under 1.1 pw max by Modeling under 1.2 pw max by Modeling under 1.3 pw max 0.5 by Modeling under 1.4 pw max by Modeling under 1.5 pw max by Modeling under 1.6 pw max 0.4 0 20 40 60 80 100 (r‐a)/(b‐a)*100 (%) Figure 5: Autofrettage hoop stress distribution under different autofrettage pressure. 150 Zhong Hu, and Sudhir Puttagunta
- 9. (r‐a)/(b‐a)*100 (%) 0.00 0 20 40 60 80 100 ‐0.05 Autofrettage Radial Stress Ratio σar/σy ‐0.10 ‐0.15 ‐0.20 ‐0.25 by Modeling by pw max ‐0.30 by Modeling under 1.1 pw max by Modeling under 1.2 pw max ‐0.35 by Modeling under 1.3 pw max ‐0.40 by Modeling under 1.4 pw max by Modeling under 1.5 pw max ‐0.45 by Modeling under 1.6 pw max ‐0.50 Figure 6: Autofrettage radial stress distribution under different autofrettage pressure. 1.4 Autofrettage von Mises Stress Ratio σai/σy 1.2 1.0 0.8 by Modeling under pw max by Modeling under 1.1 pw max by Modeling under 1.2 pw max 0.6 by Modeling under 1.3 pw max by Modeling under 1.4 pw max by Modeling under 1.5 pw max by Modeling under 1.6 pw max 0.4 0 20 40 60 80 100 (r‐a)/(b‐a)*100 (%) Figure 7: Autofrettage von Mises stress distribution under different autofrettage pressure.*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 151http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 10. When the internal autofrettage pressure is removed, the elastic deformation is trying to resumeits original shape while the plastic deformation is resisting this process so that residual stresseswithin the cylinder have been induced, and the so-called pressure autofrettage process has beenaccomplished. This unloading process basically is treated elastically. However, reverse yielding ispossible if earlier onset happens due to the Bauschinger effect. Figures 8-10 show the residualstress distribution after removed autofrettage pressure. From Figure 8, it shows a compressiveresidual hoop stress near the inner surface generated which is favorable to the thick-walled cylinderwhen it is under internal working pressure (partially cancelling the tensile hoop stress induced bythe working pressure), and a tensile residual hoop stress near the outer surface of the cylinder.Figure 9 shows a relative smaller but compressive residual radial stress left inside of the thick-wall,satisfying the boundary conditions of zero radial stress on inner surface and outer surface of thecylinder. Figure 10 shows the residual von Mises stress with higher values basically near the innersurface and outer surface of the cylinder. The turning points of the curves in Figures 8 and 10 arealmost the same as in Figures 5 and 7 indicates that the earlier onset of the reverse yielding is veryless, not changing the elastic-plastic interface very much. 0.3 Residual Hoop Stress Ratio σrθ/σy 0.2 0.1 0.0 0 20 40 60 80 100 ‐0.1 by Modeling with autofrettage of 1.1 pw max by Modeling with autofrettage of 1.2 pw max ‐0.2 by Modeling with autofrettage of 1.3 pw max by Modeling with autofrettage of 1.4 pw max ‐0.3 by Modeling with autofrettage of 1.5 pw max by Modeling with autofrettage of 1.6 pw max ‐0.4 (r‐a)/(b‐a)*100 (%) Figure 8: Residual hoop stress distribution after removed the autofrettage pressure. 152 Zhong Hu, and Sudhir Puttagunta
- 11. 0.01 (r‐a)/(b‐a)*100 (%) 0.00 Residual Radial Stress Ratio σrr/σy 0 20 40 60 80 100 ‐0.01 ‐0.02 ‐0.03 by Modeling with autofrettage of 1.1 pw max by Modeling with autofrettage of 1.2 pw max ‐0.04 by Modeling with autofrettage of 1.3 pw max by Modeling with autofrettage of 1.4 pw max by Modeling with autofrettage of 1.5 pw max by Modeling with autofrettage of 1.6 pw max ‐0.05 Figure 9: Residual radial stress distribution after removed the autofrettage pressure. 0.40 by Modeling with autofrettage of 1.1 pw max Residual von Mises Stress Ratio σri/σy 0.35 by Modeling with autofrettage of 1.2 pw max by Modeling with autofrettage of 1.3 pw max 0.30 by Modeling with autofrettage of 1.4 pw max by Modeling with autofrettage of 1.5 pw max 0.25 by Modeling with autofrettage of 1.6 pw max 0.20 0.15 0.10 0.05 0.00 0 20 40 60 80 100 (r‐a)/(b‐a)*100 (%) Figure 10: Residual von Mises stress distribution after removed the autofrettage pressure.*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 153http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 12. When an autofrettaged thick-walled cylinder is applied to an internal working pressure, thisreloading process is treated elastically, since a plastic deformation is not desired in the applicationof the cylinders based on the static yield design criterion. Figures 11-13 show the stressdistributions of an autofrettaged thick-walled cylinder after reloading by an elastic-limit pressure(i.e., the maximum working pressure 47.2 MPa). It shows more uniform distribution ofthe stress components and von Mises stress throughout the thickness of the cylinder due to theautofrettage treatment, which makes maximum von Mises stress in the cylinder less than thatwithout autofrettage treatment. However, radial stress has not been changed very much, see Figure12. Figure 14 shows the relationship of the final maximum von Mises stress versus autofrettagepressure for a thick-walled cylinder under the maximum working pressure (pw max = 47.2 MPa). Itclearly shows the optimal autofrettage pressure is about 1.5 times the maximum working pressure,and the maximum von Mises stress reduction with this autofrettage pressure is about 28%. 0.9 by Eq.(2) without autofrettage by Modeling without autofrettage by Modeling with autofrettage of 1.1 pw max by Modeling with autofrettage of 1.2 pw max 0.8 Final Hoop Stress Ratio σfθ/σy by Modeling with autofrettage of 1.3 pw max by Modeling with autofrettage of 1.4 pw max by Modeling with autofrettage of 1.5 pw max by Modeling with autofrettage of 1.6 pw max 0.7 0.6 0.5 0.4 0 20 40 60 80 100 (r‐a)/(b‐a)×100 (%) Figure 11: Final hoop stress distribution of an autofrettaged thick-walled cylinder under the maximum working pressure (pw max = 47.2 MPa). 154 Zhong Hu, and Sudhir Puttagunta
- 13. 0 Final Radial Stress Ratio σfr/σy 0 20 40 60 80 100 ‐0.05 ‐0.1 ‐0.15 by Eq.(3) without autofrettage ‐0.2 by Modeling without autofrettage by Modeling with autofrettage of 1.1 pw max ‐0.25 by Modeling with autofrettage of 1.2 pw max by Modeling with autofrettage of 1.3 pw max by Modeling with autofrettage of 1.4 pw max ‐0.3 by Modeling with autofrettage of 1.5 pw max by Modeling with autofrettage of 1.6 pw max ‐0.35 (r‐a)/(b‐a)×100 (%) Figure 12: Final radial stress distribution of an autofrettaged thick-walled cylinder under the maximum working pressure (pw max = 47.2 MPa). 1 0.9 Final von Mises Stress Ratio σfi/σy 0.8 0.7 by Eq.(5) without autofrettage 0.6 by Modeling without autofrettage 0.5 by Modeling with autofrettage of 1.1 pw max by Modeling with autofrettage of 1.2 pw max 0.4 0 20 40 60 80 100 (r‐a)/(b‐a)×100 (%)Figure 13: Final von Mises stress distribution of an autofrettaged thick-walled cylinder under the maximum working pressure (pw max = 47.2 MPa).*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 155http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 14. 1.05 Reloading Max von Mises Stress 1 0.95 0.9 σi /σy 0.85 Ratio 0.8 0.75 0.7 0.65 0.6 0.9 1.1 1.3 1.5 1.7 Autofrettage Pressure Ratio pa/pw max Figure 14: Final maximum von Mises stress versus autofrettage pressure for a thick-walled cylinder under the maximum working pressure (pw max = 47.2 MPa). 0.4 1.4E‐3 σi/σy with Bauschinger effect under 1.4 pw max σi/σy without Bauschinger effect under 1.4 pw max σi/σy with Bauschinger effect under 1.5 pw max σi/σy without Bauschinger effect under 1.5 pw max 1.2E‐3 Residual von Mises Stress Ratio σri/σy σi/σy with Bauschinger effect under 1.6 pw max Residual Equivalent Strain εri 0.3 σi/σy without Bauschinger effect under 1.6 pw max εi with Bauschinger effect under 1.4 pw max 1.0E‐3 εi without Bauschinger effect under 1.4 pw max εi with Bauschinger effect under 1.5 pw max εi without Bauschinger effect under 1.5 pw max 8.0E‐4 εi with Bauschinger effect under 1.6 pw max 0.2 εi without Bauschinger effect under 1.6 pw max 6.0E‐4 4.0E‐4 0.1 2.0E‐4 0.0 0.0E+0 0 20 40 60 80 100 (r‐a)/(b‐a)×100 (%)Figure 15: Comparison of residual von Mises stress and equivalent strain with and without the Bauschinger effect. 156 Zhong Hu, and Sudhir Puttagunta
- 15. 0.75 1.4E‐3 1.2E‐3 0.70 Final von Mises Stress Ratio σfi/σy 1.0E‐3 Final Equivalent Strain εfi 8.0E‐4 0.65 σi/σy with Bauschinger effect under 1.4 pw max 6.0E‐4 σi/σy without Bauschinger effect under 1.4 pw max σi/σy with Bauschinger effect under 1.5 pw max σi/σy without Bauschinger effect under 1.5 pw max 0.60 σi/σy with Bauschinger effect under 1.6 pw max 4.0E‐4 σi/σy without Bauschinger effect under 1.6 pw max εi with Bauschinger effect under 1.4 pw max εi without Bauschinger effect under 1.4 pw max εi with Bauschinger effect under 1.5 pw max 2.0E‐4 εi without Bauschinger effect under 1.5 pw max εi with Bauschinger effect under 1.6 pw max εi without Bauschinger effect under 1.6 pw max 0.55 0.0E+0 0 20 40 60 80 100 (r‐a)/(b‐a)×100 (%) Figure 16: Comparison of final von Mises stress and equivalent strain with and without the Bauschinger effect. Figure 15 shows the difference of the residual von Mises stress and residual equivalent strainwith or without the Bauschinger effect by modeling. It shows a difference between the results byconsidering the Bauschinger effect or not considering the Bauschinger effect, and an earlier onsetof the reverse yielding occurred by modeling with the Bauschinger effect (an earlier turning point)than that without the Bauschinger effect, especially when larger autofrettage pressure applied. Figure 16 shows the difference of the final von Mises stress and final equivalent strain with orwithout the Bauschinger effect by modeling. It shows a clear difference between the results byconsidering the Bauschinger effect or not considering the Bauschinger effect, and a earlier turning*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 157http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 16. point by modeling with the Bauschinger effect than that without the Bauschinger effect, especiallywhen larger autofrettage pressure applied, due to the previous generated elastic-plastic interfaceduring the autofrettage process. This phenomenon indicates an earlier yield may occur for aninternally pressure autofrettaged thick-walled cylinder under a working pressure by consideringthe Bauschinger effect. Therefore, in a design of safety, the Bauschinger effect should not beignored.4. Conclusions The Internal pressure overloading autofrettage processes of a thick-walled cylinder have beennumerically investigated by finite element analysis, taking into account the elasto-plastic strainhardening material with kinematic hardening (the Bauschinger effect) and the von Mises yieldcriterion. The corresponding axi-symmetric and plane-stress model has been employed. Theresidual stresses in the thick-walled cylinder induced by autofrettage pressure have beennumerically analyzed and optimized. Under the giving geometric and material condition, theoptimum autofrettage pressure has been found to be about 1.5 times the elastic-limit workingpressure, and the maximum reduction percentage of the maximum von Mises stress in theautofrettaged thick-walled cylinder under the elastic-limit working pressure has been found to beabout 28%. The Bauschinger effect does induce an earlier onset of the reverse yielding for aninternally pressure autofrettaged thick-walled cylinder under a working pressure. Therefore, in adesign of safety, the Bauschinger effect should not be ignored.5. Acknowledgements This work was supported by the State of South Dakota and Mechanical EngineeringDepartment at South Dakota State University, and inspired by the Department of Defense project(Cooperative Agreement # W15QKN-09-2-0002) by METLAB at South Dakota State University.6. References ASM International Handbook Committee. (1990). Metals Handbook, 10th ed., vol. 1, , ASM International, Materials Park, OH.Avitzur, B. (1994). Autofrettage – stress distribution under load and retained stresses after depressurization. Int. J. Pres. Ves. & Piping, 57, 271-287. 158 Zhong Hu, and Sudhir Puttagunta
- 17. Ayob, A. B., M. N. Tamin, andM. K. Elbasheer. (2009). Pressure limits of thick-walled cylinders. Proceedings of the International MultiConference of Engineers and Computer Scientists IMECS2009, Vol II, 1649-1654, March 18-20, 2009, Hong Kong.Bihamta, R., M. R. Movahhedy, and A. R. Mashreghi. (2007). A numerical study of swage autofrettage of thick-walled tubes. Materials & Design, 28(3), 804-815.Boyer, H. E., L. Timothy, and T. L Gall. (Eds.) (1985). Metals Handbook, American Society for Metals, Materials Park, OH.Bundy, M. L., P. J. Conroy, and J. L. Kennedy. (1996). Simulation & experimental in-wall temperature for 120 mm Ammunition. Defense Science Journal, 46(4), 223-232.Bush, S. H. (1988). Statistics of pressure vessels and piping failures. Journal of Pressure vessel Technology, 110, 225-233.Chu, S. C. and J. D. Vasilakis. (1973). Inelastic behavior of thick-walled cylinders subjected to nonproportionate loading. Experimental Mechanics, 113-119.Daniels, F. H. (1942). An interesting boiler explosion. Transactions of ASME, 66(2), 81-126.Darijani, H., M. H. Kargarnovin, and R. Naghdabadi. (2009). Design of thick-walled cylindrical vessels under internal pressure based on elasto-plastic approach. Materials & Design, 30(9), 3537-3544.Davidson, T. E., D. P. Kendall, and A. N. Reiner. (1963). Residual stresses in thick-walled cylinders resulting from mechanically induced overstrain. Experimental Mechanics, 3(11), 253-262.Davidson, T. E., and D. P. Kendall. (1970). The design of pressure vessels for very high pressure operation, Mechanical Behavior of Materials Under Pressure, (Pugh H L P, Ed.) Elsevier Co.Ford, H., E. H. Watson, and B. Crossland. (1981). Thoughts on a code of practice for forged high pressure vessels of monobloc design. Journal of Pressure Vessel Technology, Transactions of ASME, 103, 2-8.Gao, X-L. (1992). An exact elasto-plastic solution for an open-ended thick-walled cylinder of a strain-hardening material. Int. J. Pres. Ves. & Piping, 52, 129-144.Gao, X-L. (2003). Elasto-plastic analysis of an internally pressurized thick-walled cylinder using a strain gradient plasticity theory. International Journal of Solids and Structures, 40, 6445-6455.Gibson, M. C. (2008). Determination of residual stress distributions in autofrettaged thick-walled cylinders. Ph.D. Thesis. Granfield University April 2008.*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 159http://TUENGR.COM/ATEAS/V01/143-161.pdf
- 18. Harvey, P. D. (editor) (1982). Engineering Properties of Steels. American Society for Metals, Metals Park, OH.Hojjati, M. H., and A. Hassani. (2007). Theoretical and finite-element modeling of autofrettage process in strain-hardening thick-walled cylinders. Int. J. Pres. Ves. & Piping, 84, 310-319.Huang, X. P. (2005). A general autofrettage model of a thick-walled cylinder based on tensile-compressive stress-strain curve of a material. The Journal of Strain Analysis for Engineering Design, 40, 599-607.Iremonger, M. J. and G. S. Kalsi. (2003). A numerical study of swage autofrettage. J. Pressure Vessel Technol, 125(3), 347-351.Kandil, A. (1996). Analysis of thick-walled cylindrical pressure vessels under the effect of cyclic internal pressure and cyclic temperature. Int. J. Mech. Sci., 38(12), 1319-1332.Kihiu, J. M., S. M. Mutuli, and G. O. Rading. (2003). Stress characterization of autofrettaged thick-walled cylinders. International Journal of Mechanical Engineering Education, 31(4), 370-389.Korsunsky, A. M. (2007). Residual elastic strains in autofrettaged tubes: elastic-ideally plastic model analysis. Journal of Engineering Materials and Technology, 129, 77-81.Lazzarin, P. and P. Livieri. (1997). Different solutions for stress and stress fields in autofrettaged thick-walled cylinders. Int. J. Pres. Ves. & Piping, 71, 231-238.Malik, M. A., and S. Khushnood. (2003). A review of swage – autofrettage process. 11th International Conference on Nuclear Engineering, ICONE-11-36257 Tokyo, Japan, April 20-23, 2003, 12pages.Masu, L. M., and G. Craggs. (1992). Fatigue strength of thick walled cylinders containing cross bores with blending features. Journal of Mech. Eng. Sci., 206, 299–309.Parker, A. P., G. P. O’Hara, and J. H. Underwood. (2003). Hydraulic versus swage autofrettage and implications of the Bauschinger effect. Journal of Pressure Vessel Technology, 125, 309-314.Peckner, D. and I. M. Bernstein. (1977). Handbook of Stainless Steels. McGraw-Hill Book Company, New York, NY.Perl, M. and J. Perry. (2006). An experimental-numerical determination of the three-dimensional autofrettage residual stress field incorporating Bauschinger effects. Journal of Pressure Vessel Technology, 128, 173-178.Perry, J. and J. Aboudi. (2003). Elasto-plastic stresses in thick walled cylinders. Transactions of the ASME, 125, 248-252.Perry, J. and M. Perl. (2008). A 3-D model for evaluating the residual stress field due to swage 160 Zhong Hu, and Sudhir Puttagunta
- 19. autofrettage. Journal of Pressure Vessel Technology, Transactions of the ASME, 130, 041211-1-6.Shannon, R. W. E. (1974). Stress intensity factors for thick-walled cylinders. Int. J. Pres. Ves. & Piping, 2, 19-29.Swanson Analysis System Inc. (2011). ANSYS 13.0 User’s Manual, Houston.Tan, C. L. and K. H. Lee. (1983). Elastic-plastic stress analysis of a cracked thick-walled cylinder. Journal of Strain Analysis, 18(4), 253-260.Ugural, A. C. (2008). Mechanics of Materials, John Wiley & Sons. Inc, NJ.Venter, A. M., R. R. de Swardt, and S. Kyriacon. (2000). Comparative measurements on autofrettaged cylinders with large Bauschinger reverse yield zones. Journal of Strain Analysis, 35(6), 459-469.Zapfec, C. A. (1942). Boiler embrittlement. Transactions of ASME, 66(2), 81–126.Zhao, W., R. Reshadri, and R. N. Dubey. (2003). On thick-walled cylinder under internal pressure. Journal of Pressure Vessel Technology, 125, 267-273.Zhu, R. and J. Yang. (1998). Autofrettage of thick cylinders, Int. J. Pres. Ves. & Piping, 75, 443-446. Dr. Zhong Hu is an Associate Professor of Mechanical Engineering at South Dakota State University. He received his BS and Ph.D. in Mechanical Engineering from Tsinghua University. He has worked for railway manufacturing industry as a senior engineer, Tsinghua University as a professor, Japan National Laboratory as a fellow, Cornell University, Penn State University and Southern Methodist University as a research associate. He has authored about 70 publications in the journals and conferences in the areas of nanotechnology and nanoscale modeling by quantum mechanical/molecular dynamics (QM/MD); development of renewable energy related materials; mechanical strength evaluation and failure prediction by finite element analysis (FEA) and nondestructive engineering (NDE); design and optimization of advanced materials (such as biomaterials, carbon nanotube, polymer and composites). Sudhir Puttagunta is a graduate student in the Department of Mechanical Engineering at South Dakota State University. He holds a BS in Mechanical Engineering from Nagarjuna University, India. He is interested in mechanical design, strength analysis and computer modeling.Peer Review: This article has been internationally peer-reviewed and accepted for publication according to the guidelines given at the journal’s website.*Corresponding author (Z.Hu). Tel/Fax: +1-605-688-4817. E-mail address:Zhong.Hu@sdstate.edu. 2012. American Transactions on Engineering & AppliedSciences. Volume 1 No.2 ISSN 2229-1652 eISSN 2229-1660. Online Available at 161http://TUENGR.COM/ATEAS/V01/143-161.pdf

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment